UV Irradiation-induced Silver Nanoparticles as Mosquito Larvicides
Silver nanoparticles have a great potential for use in biological control including antimicrobial activity. The pest control of mosquito Aedes aegypti by means of larvicidal is still necessity in order to diminish the vector of some life-threaten diseases. In this study, polymethacrylate (PMA)-stabilized silver nanoparticles were synthesized by UV irradiation, characterized by Surface Plasmon Resonance (SPR), Transmission Electron Microscopy (TEM) and zeta potential measurement and evaluated for their larvicidal activity toward A. aegypti larvae. Through the processes of characterization and larvicidal assay, silver nanoparticles were spherical and in nanoscale size (= 10 nm). The larvicidal activity of silver nanoparticles was concentration-dependent and supposed to arise from the penetration of the nanoparticles into the larval membrane. The PMA-capped silver nanoparticles at a concentration of 5 ppm exhibited less than 10% survival of larvae within 3-h exposure time. The study suggests that the silver nanoparticles synthesized by UV-irradiation can be employed in biocontrol of pest including mosquito larvae.
Received: May 15, 2010;
Accepted: July 29, 2010;
Published: October 14, 2010
From the current situation of global warming and contaminated fresh water pools,
a number of mosquitoes are markedly increasing in concurrence with a high incidence
of dengue fever (Halstead, 2007). A decrease in dengue
vector breeding by using larvicides against vector Aedes aegypti (Culicidae)
is a strategy to control this pandemic life-threaten disease. The common mosquito
larvicides nowadays include an organophosphate temephos, methoprene and soil
bacterium, Bacillus thuringiensis israelensis and B. sphaericus.
However, the high amount of chemical larvicides could lead to long term residual
effect to the environment while the use of bacterial protein is in high cost
and requires a complex purification process (Aiub et
al., 2002; Pinheiro and Tadei, 2002). More importantly,
the incidences of resistance to larvicides of mosquito larvae have been reported
(Braga et al., 2004; Melo-Santos
et al., 2010). Thus, attempts to develop novel materials as mosquito
larvicides are still necessary.
Silver nanoparticles are emerging as one of the fastest growing materials due
to their unique physical and chemical properties, small size and high specific
surface area. They can be employed in material and engineering such as microelectronic
(Zhang et al., 2005), catalyst (Wang
et al., 2005), biosensor (Frederix et al.,
2003) and in biomedicine especially for antibacterial agent (Lok
et al., 2006; Panacek et al., 2006;
Kim et al., 2007; Shrivastava
et al., 2007; Choi et al., 2008;
Guzman et al., 2008; Rai
et al., 2009) and antiviral agent (Elechiguerra
et al., 2005). Silver nanoparticles can be synthesized by using chemicals
such as sodium borohydride for reduction of divalent silver atom to zerovalent
silver atom (Solomon et al., 2007). Recently,
an alternative of green chemistry to silver synthesis becomes more attractive
since the remediation of environmental toxic waste is unnecessary. The silver
nanoparticles capped with polymethacrylic acid (PMA) and produced by UV irradiation
was previously synthesized (Dubas and Pimpan, 2008;
Spadaro et al., 2009) and used for sensing application
(Dubas and Pimpan, 2008). The biocompatibility and harmlessness
of the PMA polymer make it appropriate to be employed in biomedical application
(Li and Lee, 2009). Accordingly, the use of PMA-capped
silver nanoparticles synthesized by photoreduction for larvicidal activity towards
A. aegypti is our objective for this study.
MATERIALS AND METHODS
Chemicals: Polymethacrylic acid (PMA) was purchased from Sigma-Aldrich (USA). Silver nitrate (AgNO3) and temephos (O,O,O',O'-tetramethyl-O,O'-thiodi-p-phenylene diphosphorothioate) were supplied from Carlo Erba, Italy and Chemfleet, Thailand, in orderly. The acetic-acetate buffer (pH = 4.75) was prepared by mixing equal volumes of 10 mM acetic acid (Sigma-Aldrich, USA) and 10 mM sodium acetate (Riedel-de Haen AG, Switzerland) solutions.
Synthesis of silver nanoparticles: The UV irradiation-induced silver
nanoparticles were synthesized by previously described method (Dubas
and Pimpan, 2008). The 10 mM PMA in 10 mM acetic-acetate buffer solution
at a volume of 25 mL was added to another 25 mL of 10 mM AgNO3 in
10 mM acetic-acetate buffer solution. The mixture was stirred at room temperature
for 5 min before exposed to low intensity (8 W) UV lamp for approximately 90
min. The solution of synthesized silver nanoparticles appeared in deep purple
color and contained 540 ppm of Ag atom.
Characterization of silver nanoparticles: The nanoparticles were characterized for surface plasmon resonance (SPR) by UV-Visible spectroscopy (Specord S100, Analytikjena, Germany). The morphology and particle size of nanoparticles were visualized by Transmission Electron Microscopy (TEM) (H-7650, Hitachi, Japan). The surface charges of the particles were measured at 25°C using a zetasizer apparatus (NanoZS, Malvern, UK).
Larvicidal activities of silver nanoparticles
Culture of mosquito larvae: The larval culture was done on A.
aegypti eggs obtained from Department of Parasitology, Faculty of Medicine,
Chulalongkorn University, Bangkok, Thailand. To start the colony the larvae
were hatched and reared in plastic cups containing dechlorinated tap water at
room temperature. Mosquito larvae were fed with powdered nutrient broth once
a day. After 4 days the hatched larvae turned into larvae in early fourth larval
stage and were subjected to be employed in further experiment.
Larvicidal test: Mosquito larvae were placed in 8 batches of 20 larvae each in plastic cups containing 100 mL of the test solutions which were dilute PMA-capped silver nanoparticles at various concentrations, 0.01, 0.1, 1 and 5 ppm Ag atom. The solutions of 1 ppm AgNO3 and 1 ppm PMA were also studied for comparison. The tap water was used as a negative control (0% mortality of larvae) while the positive control (100% mortality of larvae) was the commercial larvicide, 1 ppm temephos solution. A number of dead larvae in each batch were counted every hour for 24 h exposure period. After soaked with ethanol, xylene and permount agent for each 15 min, the treated larva was mounted on a slide and examined under a microscope (Meiji EMZ-TR, Japan) for image capture on a DS-Fi1 digital camera (Nikon, Japan). Moreover, the effect of silver nanoparticles on the hatchability of A. agypti eggs was determined by hatching a hundred of eggs in plastic trays containing either water or 5 ppm silver nanoparticles and after 2 days, the newborn larvae were observed.
Synthesis and characterization of silver nanoparticles: The PMA-capped
silver nanoparticles synthesized by photoreduction were in purple color with
a corresponding absorption peak at 525 nm (Fig. 1a). The TEM
image of silver nanoparticles illustrated the uniform distribution of spherical
particles with approximately 5-10 nm in diameter (Fig. 1b).
The zeta potential of -27.7±3.07 mV represented the negative charges
of PMA stabilizer surround the particles.
Larvicidal bioassay: The effectiveness of silver nanoparticles as mosquito
larvicides was determined from a number of live larvae with exposure time periods
(Fig. 2). From the result, PMA-capped silver nanoparticles
at concentrations of 0.01 and 0.1 ppm caused no death of larvae. The nanoparticles
at 1 ppm slightly decreased the survival of larvae to 88±11% after 24
h exposure while more than 90% of mortality was observed in larvae after in
contact with 5 ppm silver nanoparticles for 3 h. The solution of 1 ppm silver
nitrate gradually killed the larvae over the experimental period and approximately
less than 10% survival was found after 17 h.
|| (a) The appearance and UV spectrum and (b) the TEM image
of PMA-capped silver nanoparticles
The survival percentage of mosquito larvae after exposure
to different concentrations of silver nanoparticles (silver nano), 1 ppm
silver nitrate and 1 ppm PMA solutions (Mean±SD, n = 20)
In contrast, the PMA solution at
the same concentration as silver nitrate was harmless to larvae. The dose of household use of 1 ppm temephos solution (positive control) could
completely eradicate all the larvae within 3 h. The 40X magnification photos
of the abdomen part of the dead larva were viewed under microscope as shown
in Fig. 3a and b. The morphology of nanoparticle-treated
larva was almost the same with untreated (water) larva except for some dark
spots appeared throughout the larval body. Moreover, the spots were not observed
in the larval body when exposed to silver nitrate or temephos solutions (data
||The 40X magnificent image of abdomen part of Aedes aegypti
larva (a) after untreated and (b) treated with 5 ppm silver nanoparticles
For hatchability assessment, it was found that there were a number
of mosquito eggs hatched in solution of silver nanoparticles, however the newborn
larvae were killed immediately after exposed to the nanoparticles.
Since silver nanoparticles are considered to be potential for biological applications
including antibacterial agent with no bacterial resistant effect, we intend
to evaluate whether they could apply for mosquito larvicidal agent. The nanoparticle
synthesis is important as the instability or aggregation of nanoparticles would
lead to a decrease in their biological activities (Kvitek
et al., 2008). In contrast to a conventional method for synthesis
of silver nanoparticles in which many reagents are required, the solely use
of UV irradiation can reduce the silver ion for nucleation of nanoparticle formation
and promote the cross-linking of the PMA polymer (Spadaro
et al., 2009). The optical properties of purple color and SPR band
at 525 nm of UV-induced silver nanoparticles gained from this study differed
from those of silver nanoparticles prepared using chemical reduction method
which were yellow with SPR band around 400-420 nm (Solomon
et al., 2007). The findings were not unexpected since the excess
PMA stabilizer was able to form Ag-PMA coordination reaction leading to dielectric
change of the medium surround the particles and a red shift in absorbance (Dubas
and Pimpan, 2008; Spadaro et al., 2009).
The estimated size (5-10 nm) of silver nanoparticles from TEM study was similar
to the size of 9.2 nm, obtained from a relationship between the full-width of
half-maximum of the absorption peak (FWHM, in nm) and the particle diameter
(D, in nm), which is FWHM = 50 + (230/D) (Choi et al.,
For the larvicidal bioassay, the dose-dependent effect of silver nanoparticles
on the mortality of the larvae was seen. The silver nanoparticles at concentrations
of 0.01, 0.1 and 1 ppm were unlikely to act as larvicidal agent toward A.
aegypti. The anionic PMA stabilizer was previously reported to be safe (Li
and Lee, 2009) which was in agreement with our study in that none of the larvae
were killed by the PMA solution. The larvicidal effect of PMA-capped silver
nanoparticles was more obvious at higher dose (5 ppm) than that of silver nitrate
solution (1 ppm). The similar finding was observed for antimicrobial activity
in that silver nitrate had a lower inhibitory concentration than that of silver
nanoparticles (Choi et al., 2008; Kvitek
et al., 2008).
For PMA-capped nanoparticles, it seemed not the case that nanoparticles markedly
interacted with the biological membrane which is negatively charged. The antibacterial
activity of silver nanoparticles previously reported was possibly due to a high
surface area of the nanoparticles especially those in a range of 10-20 nm which
provided a better contact between nanoparticles and cell (Sondi
and Salopek-Sondi, 2004; Panacek et al., 2006).
According to the average of 5-10 nm PMA-capped silver nanoparticles, we then
speculate that the mechanism which causes the death of larva is the ability
of the nanoparticles to penetrate through the larval membrane. The dark spots
inside the larval body as seen from a microscope could be presumed to be the
silver nanoparticles that agglomerated to form the clusters since they were
not found in the larvae untreated with nanoparticles.
The silver nanoparticles in the intracellular space can bind to sulfur-containing
proteins or phosphorous containing compound like DNA, leading to the denaturation
of some organelles and enzymes (Sondi and Salopek-Sondi,
2004; Choi et al., 2008; Rai
et al., 2009). Thereafter, the dropping of membrane permeability
and disturbance in proton motive force required for ATP construction are induced
which cause the lost of cellular function and finally cell death (Lok
et al., 2006). Although, 1 ppm temephos solution exhibited the similar
effect to 5 ppm silver nanoparticles in which it could get rid of all the mosquito
larvae within 3 h, its mechanism of action is different. The temephos is an
organophosphate pesticide which inhibits the hydrolysis of acetylcholine in
neuron. The accumulation of acetylcholine in neuromuscular synapse causes the
death of larvae by depression of respiratory system (Aiub
et al., 2002; Braga et al., 2004).
For silver ion (AgNO3), the larvicidal mechanism is proposed to
be the same as the nanoparticles but more focus on penetration promoted by the
attraction of positive silver ion and the cell membrane (Choi
et al., 2008; Kvitek et al., 2008).
In spite of more toxicity to living cells of silver ion than silver nanoparticles,
the drawback that limits the use of silver ion is the cause of argyria (Fung
and Bowen, 1996). When used as antibiotics, few incidences of bacterial
resistance to silver nitrate were seldom reported while none were found for
silver nanoparticles (Kvitek et al., 2008). Additionally,
silver nanoparticles had no inhibitory effect on hatchability of mosquito eggs
of A. aegypti. It might arise from the fact that the mosquito egg shell
contains chitinized serosal cuticle which can resist penetration of silver nanoparticles
(Rezende et al., 2008).
Silver nanoparticles could be environmental friendly synthesized by UV irradiation method. The PMA-capped silver nanoparticles showed the potential as an alternative to organophosphate larvicidal agent for A. aegypti. An ability to penetrate through the living organism of silver nanoparticles leading to loss of cell function is considered as a mechanistic action for death of larvae. The advantageous point of silver nanoparticles as larvicides is that the drug resistance due to the overuse of pesticides can be overcome.
The authors are grateful to Assc. Prof. Padet Siriyasatien, Department of Parasitology,
Faculty of Medicine, Chulalongkorn University for providing necessary material
and suggestion. The partially financial support from the Faculty of Graduate
Studies, Chulalongkorn University is acknowledged.
1: Aiub, C.A.F., E.C.A. Coelho, E. Sodre, L. F. R. Pinto and I. Felzenszwalb, 2002. Genotoxic evaluation of the organophosphorous pesticide temephos. Genet. Mol. Res., 101: 159-166.
Direct Link |
2: Braga, I.A., J.B.P. Lima, S.S. Soares and D. Valle, 2004. Aedes aegypti resistance to temephos during 2001 in several municipalities in the states of Rio de Janeiro, Sergipe and Alagoas, Brazil. Mem. Inst. Oswaldo Cruz., 99: 199-203.
3: Choi, O., K.K. Deng, N.J. Kim, L. Ross Jr., R.Y. Surampalli and Z. Hu, 2008. The inhibitory effects of silver nanoparticles, silver ions and silver chloride colloids on microbial growth. Water Res., 42: 3066-3074.
4: Dubas, S.T. and V. Pimpan, 2008. Green synthesis of silver nanoparticles for ammonia sensing. Talanta, 76: 29-33.
5: Frederix, F., J.M. Friedt, K.H. Choi, W. Laureyn and A. Campitelli et al., 2003. Biosensing based on light absorption of nanoscaled gold and silver particles. Anal. Chem., 75: 2894-6900.
6: Fung, M.C. and D.L. Bowen, 1996. Silver products for medical indications: Risk-benefit assessment. Clin. Toxicol., 34: 119-126.
7: Guzman, M.G., G. Dille and S. Godet, 2008. Synthesis of silver nanoparticles by chemical reduction method and their antibacterial activity. World Acad. Sci. Eng. Tech., 43: 357-364.
Direct Link |
8: Halstead, S.B., 2007. Dengue. Lancet, 370: 1644-1652.
CrossRef | Direct Link |
9: Kim, J.S., E. Kuk, K.N. Yu, J.H. Kim and S.J. Park et al., 2007. Antimicrobial effects of silver nanoparticles. Nanomed. Nanotechnol. Biol. Med., 3: 95-101.
CrossRef | Direct Link |
10: Kvitek, L., A. Panacek, J. Soukupova, M. Kolar and R. Vecerova et al., 2008. Effect of surfactant and polymers on stability and antibacterial activity of silver nanoparticles (NPs). J. Phys. Chem., 112: 5825-5834.
11: Li, Y. and M.L. Lee, 2009. Biocompatible polymeric monoliths for protein and peptide separations. J. Sep. Sci., 32: 3369-3378.
12: Lok, C.N., C.M. Ho, R. Chen, Q.Y. He and W.Y. Yu et al., 2006. Proteomic analysis of the mode of antibacterial action of silver nanoparticles. J. Proteome Res., 5: 916-924.
CrossRef | PubMed |
13: Melo-Santos, M.A.V., J.J.M. Varjal-Melo, A.P. Ara˙jo, T.C.S. Gomes and M.H.S. Paiva et al., 2010. Resistance to the organophosphate temephos: Mechanisms, evolution and reversion in an Aedes aegypti laboratory strain from Brazil. Acta Trop., 113: 180-189.
14: Panacek, A., L. Kvitek, R. Prucek, M. Kolar and R. Vecerova et al., 2006. Silver colloid nanoparticles: Synthesis, characterization and their antibacterial activity. J. Phys. Chem. B, 110: 16248-16253.
CrossRef | PubMed | Direct Link |
15: Pinheiro, V.C.S. and W.P. Tadei, 2002. Evaluation of the residual effect of temephos on Aedes aegypti (Diptera, Culicidae) larvae in artificial containers in Manaus, Amazonas State, Brazil. Cad. Saude Publica, 18: 1529-1535.
16: Rai, M., A. Yadav and A. Gade, 2009. Silver nanoparticles as a new generation of antimicrobials. Biotechnol. Adv., 27: 76-83.
CrossRef | Direct Link |
17: Rezende, G.L., A.J. Martins, C. Gentile, L.C. Farnesi, M. Pelajo-Machado, A.A. Peixoto and D. Valle, 2008. Embryonic desiccation resistance in Aedes aegypti: Presumptive role of the chitinized serosal cuticle. BMC Develop. Biol., 8: 182-182.
18: Shrivastava, S., T. Bera, A. Roy, G. Singh, P. Ramachandrarao and D. Dash, 2007. Characterization of enhanced antibacterial effects of novel silver nanoparticles. Nanotechnology, Vol. 18, No. 22. 10.1088/0957-4484/18/22/225103
19: Mulfinger, L., S.D. Solomon, M. Bahadory, A.V. Jeyarajasingam, S.A. Rutkowsky and C. Boritz, 2007. Synthesis and study of silver nanoparticles. J. Chem. Educ., 84: 322-322.
CrossRef | Direct Link |
20: Sondi, I. and B. Salopek-Sondi, 2004. Silver nanoparticles as antimicrobial agent: A case study on E. coli as a model for Gram-negative bacteria. J. Colloid Interface Sci., 275: 177-182.
CrossRef | Direct Link |
21: Spadaro, D., E. Barletta, F. Barreca, G. Curro and F. Neri, 2009. PMA capped silver nanoparticles produced by UV-enhanced chemical process. Appl. Surf. Sci., 255: 8403-8408.
22: Wang, A.Q., C.M. Chang and C.Y. Mou, 2005. Evolution of catalytic activity of Au-Ag bimetallic nanoparticles on mesoporous support for CO oxidation. J. Phys. Chem. B., 109: 18860-18867.
23: Zhang, J., X. Li, X. Sun and Y. Li, 2005. Surface enhanced Raman scattering effects of silver colloids with different shapes. J. Phys. Chem. B., 109: 12544-12548.
24: Elechiguerra, J.L., J.L. Burt, J.R. Morones, A. Camacho-Bragado, X. Gao, H.H. Lara and M.J. Yacaman, 2005. Interaction of silver nanoparticles with HIV-1. J. Nanobiotechnol., Vol. 3. 10.1186/1477-3155-3-6